REVISED APRIL 1955 INFORMATION CIRCULAR 4 The Soaking Method for the Preservative Treatment of Fence Posts By Robert D. Graham 4 OREGON FOREST PRODUCTS LABORATORY State Board of Forestry and School of Forestry, Oregon State College, Cooperating Corvallis OREGON FOREST PRODUCTS LABORATORY was THE established by legislative action in 1941 as a result of active interest of the lumber industry and forestryminded citizens. It is associated with the State Board of Forestry and the School of Forestry at Oregon State College. An Advisory Committee composed of men from representative interests guides the research program that is directly pointed toward the fuller utilization of Oregon's forest resources. The following men constitute the present membership of the Advisory Committee: PAUL PATTERSON, Governor ROBERT W. C0wLIN CHARLES W. Fox NILs HULT . . . . . .Chairman Pacific Northwest Forest and Range Experiment Station . Oregon Plywood Interests Willamette Valley Lumbermen's Association WILLIAM I. WEST. . School of Forestry CABS. A. RASMUSSEN Western Pine Association WILLIAM SWINDELLS West Coast Lumbermen's Association GEORGE SPATJR, State Forester . . Secretary Information Circular 4 Revised April 1955 The Soaking Method for the Preservative Treatment of Fence Posts By Robert D. Graham In Charge, Wood Preservation Oregon Forest Products laboratory A Release of the Oregon Forest Products Laboratory Corvallis, Oregon Table of Contents Page Summary 5 Causes of Post Failure 6 Objectives of Preservative Treatments 6 Factors Affecting Treatment 6 Anatomical Structure 6 Penetration of Preservative Solution 7 Treatability and Durability of Heartwood and Sapwood 12 Moisture Content 14 Seasoning Conditions 14 Treating Conditions 14 Preparation of Posts for Treatment Cutting and Peeling 15 15 Incising 15 Seasoning 16 The Soaking Method 17 Equipment 17 Preservatives 18 Control of Treatment 19 Treating Standards 19 Cost of Treating Solution 20 Handling Preservative-treated Posts 21 Advantages of Preservative-treated Posts 21 Appendix Service Life of Untreated Posts in the T. J. Starker Post Farm 22 Selected References on Wood Preservation 23 Partial List of Manufacturers and Distributors of Copper Naphthenate and Pentachlorophenol Commercial Wood Preserving Plants in Oregon 25 26 Treated foundation posts for seasoning rack. Incised, seasoned Douglas fir posts were soaked in a preservative-diesel oU solution using the re- versing-end method and a soaking time of 6 days for each end. The penetrations are outlined in black. Very nearly complete sapwood penetration was obtained. The average retention of the 60 posts in the charge was 2.9 pounds per cubic foot. The Soaking Method for the Preservative Treatment of Fence Posts SUMMARY The soaking method for the preservative treatment of fence posts consists of immersing seasoned, preferably incised, wood posts in preservative solutions to the desired depth for a sufficient length of time to secure a uniformly treated outer shell of wood. Watersoluble and oil-soluble preservatives may be used, but under the severe service conditions to which fence posts are subjected, watersoluble preservatives may be leached quite rapidly from the wood. For this reason, the discussion has been limited largely to the more permanent oil-soluble preservatives. The soaking method can be used successfully for the preserva- tive treatment of the sapwood of many Oregon tree species. Posts properly treated should provide a useful service life of 15 years. The results attained by this method will depend largely on the care with which the material is prepared for treatment and, at best, cannot be expected to compare with those of pressure processes in which higher preservative retentions and deeper penetrations are obtained. For best results, the following procedure for preparing and treating posts is recommended: Slope the tops of the posts as they are cut. Separate the posts by species as they are peeled. Incise the posts to a depth of at least one-half inch. Season the posts until splits and checks open. Include only posts of one species and one seasoning condition in each treating charge. Inspect the posts to determine when treatment is complete. Avoid exposing untreated wood during subsequent handling. Marked variations in the receptiveness of the material to treatment and the wide range in seasoning conditions make it virtually impossible to establish definite treating schedules for any species. A selected list of references on wood preservation, and a list of commercial treating plants in Oregon, are included in the Appendix for those who may wish to purchase treated material or to delve into the various aspects of the preservation of wood. INFORMATION CIRCULAR 4 6 CAUSES OF POST FAILURE Fence posts and other wood products in cOntact with the ground are subject to severe and virtually continuous attack by wood-destroying organisms and to the constant effects of mechanical and chemical deterioration. Destruction of the wood is accelerated greatly at the ground-line zone (about 6 inches above to 12 inches below the ground level) where moisture, air, and temperature conditions favorable to insects and fungi prevail. It is in this section that fungus and insect attacks usually begin. Also, in this zone preservatives are most subject to removal by leaching and by mechanical erosion of the outer layers of the treated wood. Deterioration may begin in the tops of the posts under moist climatic conditions, although the rate of deterioration is usually much slower than in the ground-line section. The sides of the posts above the ground-line zone are least subject to deterioration. OBJECTIVES OF PRESERVATIVE TREATMENTS Preservative treatment with proper toxic chemicals renders wood resistant to insect or fungus attack. Since it is seldom possible or economically feasible to impregnate wood completely, the treatment is more or lessretricted to an outer layer of wood (Frontispiece), which thust be treated uniformly to a depth sufficient to withstand the continuous action of the many agencies of deterioration. FACTORS AFFECTING TREATMENT The preservative treatment of wood is influenced by numerous factors that determine the limitations of the method employed and explain the great variations in the penetration and retention of the preservative solution. Anatomical structure The stem of a tree, when crosscut and viewed from the end, reveals several distinct features. These include, in order of their occurrence towards the center of the tree, the outer bark, inner bark, sapwood, heartwood, and pith. The outer bark serves as a protective covering to prevent mechanical damage and evaporation of water. The thin inner bark serves to distribute food, which has been manufactured in the leaves, to a single layer of growing cells that produce new wood and new inner bark. The sapwood, consisting of living, dying, and dead cells, conducts soil nutrients in water solution to the leàtres for conversion into food for cell growth. The wood of young trees may be composed entirely of sapwood. The heartw'ood, THE SOAKING METHOD FOR PRESERVING FENCE POSTS which once was sapwood, consists of dead cells. Because of the extractives it contains, it is often much darker in color than sapwood. The pith, usually found near the center of the cross section of the tree trunk, consists of a small core of cells that serve to store food, particularly for the growing tips of the stem and branches. The wood of trees grown in temperate climates contains annual rings. Cell growth in such climates is not continuous because trees are dormant in the winter. This discontinuity of growth produces the annual rings, each of which has two parts, the springwood and the summerwood. The springwood, which is formed during the early part of the growing season, is composed of relatively large thinwalled cells, but the later-formed summerwood consists of smaller, thick-walled cells. Wood is composed of many types of cells that vary greatly in size and structure. The hardwoods (Figure 1) contain more kinds of cells than the softwoods (Figure 2). The softwoods principally contain tracheids, commonly called fibers, which conduct nutrients and strengthen the stem, and special cells (wood rays) for the distri- bution and storage of food. Some have resin canals (intercellular spaces) that may or may not be plugged with resin. The hardwoods have similar cells for the storage of food, but they have specialized for the conduction of nutrients (vessels or pores) and for strength (fibers). The vessels may be fairly uniform in size and well distributed throughout the wood, as in alder or maple, or they may vary greatly in size, the largest ones being conftned to the cells springwood, as in oak and ash. These vessels form nearly continuous vertical openings in the wood, though in some species, such as white oak, they may he plugged with cyst-like structures, called tvloses. Moisture and food materials pass from one cell to another through thin places in the cell walls. These thin places are called pits. Summerwood cell walls have fewer and smaller pits than those of the springwood. Penetration of preservative solutions The preservative solution may penetrate the wood through unplugged resin canals and vessels, pits, small checks in the cell wall, and directly through the cell wall. The rate of penetration is affected b the size and number of the various cell structures and by the thickness and permeability of the cell walls. As the longest axes of most of the cells are in a vertical plane, the penetration will be more rapid in this longitudinal direction because of he smaller number of cell walls through which the preservative must pass. Longitudinal Uniseriate Ray 0 0 x 0 0 0. bark 0 bark Cl, Outer Inner Springwood nrna Vessel or Pore V V 0 5 V do I- .:I, V )VQ0 thick-walle 0 CRadial section. u- section. BTangential section. ray in the - wing four Sketch showing the relative positions of the wood sections from which the photographs were taken. ACross Parenchyma Fibers Vessel - -. a-----. , . .-i;,Lf -spr --- 9 - ---. and into of B. Tangential section showing uniseriate wood rays interspersed among thick-walled wood fibers and thinV -Q 0 0 '.Q V -C Figure 1. Gross features and anatomical structure of White oak. (PhotographsX 100) C B 0 walled parenchyma. Wood Rays a. 0 0 0 0 bark bark V 0 0 Outer Inner -. 'S SS, i 'I '.% - 0 ou showing resin ducts in an annual ring, in the thickness of the tracheids within and the thin-walled tracheids of the th. Summerwood Springwood -V .%!%%'4%..O.,.S.sj ;s......a..S :::V..',.,,. es i ;I :: ""S S I I SSSS 4I l's "' ' I%$$SSSSSS S- CRadial section. sewsea 4 BTangential section. 5 section. '' a Sketch showing the relative positions of the wood sections from which the photographs were taken. ACross S...., -.. ' ';: . O.,,*bflS$55%1 UI 0 0 0' C a. C,) Summerwood Tracheids utTht Ray Tracheids Springwood Wood Ray B. Tangential section showi ng uniseriate wood rays and one fusiform wood ray co ntaining a horizontal resin duc interspersed among the tracheids. The fine lines are spiral thickenings on the walls of the tracheids. C. Radial section showing a wood ray extending through summerwood into the springwood. The numerous cir- des are bordered pits in the walls of the tracheids. Figure 2. Gross features and anatomical structure of Douglas fir. (PhotographsX 100) 12 INFORMATION CIRCULAR 4 penetration has been estimated to be from 7 to more than 25 times as great as radial penetration (across the annual rings) or tangential penetration (around an annual ring). The longitudinal penetrations in the sapwoods of several species are indicated in Table 1. Radial penetration is quite rapid in pine, but slow in Douglas fir and Western larch. End penetration is rapid in many hardwoods. Table 1. SOAKING PERIODS TO BE USED AS A GUIDE FOR TREATING THE SAPWOOD OF INCISED, SEASONED POSTS WITH A PRESERVATIVE- DIESEL OIL SOLUTION Top Longitudinal penetration in sapwood after a 24-hour soak* Hours Inches Soaking period Species Alder, red Aspenf Cedar, western redt Cottonwood, black Douglas fir Fir, whitef Larch, Western Hours 6-24 6-24 24-48 6-24 48-144 48-96 48-96 6-24 48-144 6-72 2-6 2-6 16-22 8-24 2-6 24-48 24-48 24-48 2-6 24-48 2-6 Maple, bigleaf Oak, Oregon white. Pine, lodgepolef * Immersion depth 26 to 30 inches. t Based in part on the publication Cold-Soak Wood Preservation by Ernest Wohletz and Vernon Ravenscroft. Glaze, strips of bark, and other surface conditions may interfere seriously with radial penetration, producing a thin irregularly treated shell of wood. The exposure of end grain by incising helps to eliminate the effects of these surface conditions by permitting end penetration, which increases preservative retention and reduces the treating time required to obtain a uniformly deep treatment. The distribution of a preservative-diesel oil solution from the butt and from an incision at the ground line is shown in Figure 3. The limitations of the painting method are clearly illustrated in Figure 4. Although a somewhat better treatment might be obtained in other species, virtually no penetration and no adequate retention can be obtained by this method of applying oil-borne preservatives. Treatability and durability of heartwood and sapwood The formation of heartwood in most trees is characterized by a darkening in color and the presence of extractives, some of which may inhibit development of wood-destroying organisms, but which THE SOAKING METHOD FOR PRESERVING FENCE POSTS 13 may also interfere seriously with the penetration of the preservative. The sapwood, although naturally less durable, is generally easier to treat. For this reason, the soaking and other nonpressure methods Figure 3. Penetration of preservative in Douglas fir. Douglas fir post sections were seasoned to 12 per cent moisture content, cut half- way through at 24 inches from the butt end, and soaked for different periods of time. Penetrations are indicated by black lines. Figure 4. Douglas fir posts painted with wood preservatives. The posts were given two heavy coats of the preserva- tives. Each coat was applied on a different hot summer day. Virtually no penetration was obtained and no increase in service life can be expected. are limited to the treatment of the sapwood. Round posts of all species should be treated. Split posts containing durable heartwood and appreciable amounts of sapwood also should be treated, though little or no increase in the service life of the heartwood can be ex- INFORMATION CIRCULAR 4 14 pected from the treatment. Thick sapwood permits deeper penetration and higher retentions of the preservative solution. The relative durabilities of a number of Oregon woods are listed in the Appendix. These values represent maximum rather than typical serviceability, for the posts from which these test data were collected are not subject to the nailing, groundline erosion, and physical forces that frequently reduce the service life of posts actually in use. For example, several untreated cedar series in the test indicate a service life in excess of 20 years; in actual use, the service life of cedar posts is about 12 years. Moisture content Wood treats much more readily at a moisture content of less than 20 per cent when oil-soluble preservativs are used. Low moisture content also prevents reduction of the concentration of the preservative in the wood when water-soluble preservatives are employed. The moisture content of freshly cut sapwood is high, frequently exceeding 150 per cent (oven-dry basis), but it can be reduced to 16 per cent or less in a few summer months when proper seasoning practices are employed. Posts at a moisture content suitable for treating will have numerous checks, will be lighter in weight, and will feel dry to the touch. Seasoning conditions Weather and the length of the seasoning period have a marked effect on surface conditions, seasoning checks, and drying rate of posts. Overwintering has been suggested for the elimination of glaze on lodgepole pine, but precautions must be taken to prevent attack by wood-destroying organisms. The advantages to be gained from long seasoning periods are not fully established. In general it appears that the best results will be obtained if posts are peeled, seasoned, and treated in the same year. Treating conditions Dry, warm, or hot weather favors penetration of the preservative by maintaining the treating solution at a minimum viscosity and by insuring that the surface of the material to be treated is relatively free of moisture. Penetration improves as the viscosity of the solution decreases, but lower viscosity oils evaporate more rapidly and are usually more inflammable and more expensive. The lower viscosity diesel oils are satisfactory for treating most species, but it should be possible to use higher viscosity oils for treating incised posts of species that are easy to treat. In any case, the preservative must be sufficiently soluble in the oil to secure the required preservative concentration. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 15 The practice of adding water to raise the level of the preservative-oil solution above the butt ends of the posts to reduce retention is not recommended. It serves no useful purpose in treating posts of thin sapwood species or species that are difficult to treat. In posts of easily treated species, longitudinal penetration of the water may be so rapid as to interfere seriously with the radial penetration of the preservative in the ground-line zone, and the increased weight of the post will give an erroneous indication of the amount of preservative retained. PREPARATION OF POSTS FOR TREATMENT The success attained by the soaking method and the serviceability of the treated product will be determined largely by the man- ner in which the posts are prepared for treatment. Every effort should be made to prepare the posts so that it will not be necessary to cut them after they are treated. Cutting and peeling Posts cut in the spring and early summer will peel more readily and season enough to be ready for treatment in late summer or early fall. They should be peeled, the butts of posts to be driven should be pointed, the tops should be sloped, and they should be incised and piled for seasoning immediately after cutting in order to promote drying and to discotrage attack by wood-destroying organisms. Peeling may be done with an axe, a flat-bladed shovel, a barking spud, a drawknife, or an old shovel worn to a "V." Incised posts need not be peeled clean, though strips of bark that might interfere with seasoning or with the depth of the incision should be removed. Incising The incisions may be distributed uniformly over the surface of the post, or they may be made in rings of staggered incisions. Particular attention should be paid to incising the ground-line zone to insure a uniformly deep penetration in this critical area. The incisions may be made with an axe blade (Frontispiece), saw, incising hammer, or with incising blades mounted on the head of an axe. The last two incising devices and their respective incising patterns are shown in Figure 5. The incisions should be staggered to minimize reduction in the strength of the post. Although some of the incisions may seem severe, after a few years of service the loss in strength will be much less than that caused by wood-destroying organisms in untreated posts. The distance between incisions will depend on the species being 16 INFORMATION CIRCULAR 4 for A multipointed incising hammer and incising blades attached to the head of an axe. The points and blades should be made of heat-treated tool steel for long service. treated and on the soaking time to be employed. Table 1 Can be used as a guide in estimating this distance. For example, the incisions in alder, cottonwood, and maple may be from 8 to 12 inches apart for a 24-hour soaking period, while the incisions in Douglas fir should be not more than 6 inches apart for a 96-hour soaking period. A large number of small incisions will facilitate a higher preservative retention than will a small number of large incisions. Seasoning Seasoning reduces the moisture content of the wood, and the resultant shrinkage causes the wood to split and check. Moderate checking is desirable, for this permits treatment of wood that otherwise would be exposed if unchecked treated posts were to continue to season after their installation. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 17 The posts should be cross-piled on stone or sound wood supports at least 18 inches above ground to provide good circulation under and throughout the seasoning pile. Grass, brush, or weeds should be cleared from under and around the seasoning pile, for they will interfere with circulation and may promote conditions favorable to wood-destroying organisms. Under normal summer conditions, posts from 4 to 6 inches in diameter can be seasoned in 1 to 3 months, but the seasoning period will vary with the size of the posts and with local climatic conditions. The rate of seasoning can be controlled to some extent by varying the spacing between individual posts and between layers of posts in the pile. In dry hot climates where the rate of seasoning is very rapid, the posts may be placed closer together, and the seasoning piles should be located out of the direct rays of the sun to reduce the rate of seasoning and thus prevent the development of large splits or checks. THE SOAKING METHOD This method consists of soaking the material in a preservative solution for a sufficient length of time to obtain the required penetration of the solution. Penetration can be controlled to a large extent by incising the posts to the desired depth and by soaking them for a sufficient length of time to treat completely the wood between the incisions. Posts can be treated in either a horizontal or a vertical position. Large timbers can best be treated in the horizontal position, and the treating tanks should be equipped with devices for keeping the timbers submerged. Standing posts on end in tanks slightly deeper than one-half the length of the posts and then reversing the ends will permit some control of preservative retention in the butts and the tops of the posts. Equipment Oil-tight tanks or drums with covers are the only equipment required, though more elaborate equipment can be used for permanent or semipermanent installations. Ordinary 55-gallon drums are excellent if the posts are to be treated by the reversing-end method. Each drum will hold about 13 posts from 4 to 6 inches in diameter and will require about 20 gallons of treating solution to raise the liquid level to 30 inches. The drums are 22 inches in diameter and 34 inches deep. Tanks for treating long material can be made by welding together two or more drums and burying the unit in the ground to 18 INFORMATION CIRCULAR 4 a convenient working level. The tanks should be equipped with covers to prevent accumulation of water in the bottom during wet weather. Deeper tanks will require devices for keeping the material submerged during treating. Preservatives Either oil-soluble or water-soluble preservatives may be used, although the former are generally more permanent. However, a new double-diffusion process* may provide a relatively permanent waterborne preservative treatment. Coal-tar creosote is an excellent preservative and should prove satisfactory when diluted about 50 per cent in volume with low-viscosity oils. Oil-gas-tar creosotef also should prove satisfactory. Two oil-soluble preservatives, pentachiorophenol and copper naphthenate, are well suited to the soaking method. Both are sold in concentrated and ready-to-use solutions. The concentrates are easy to store, are readily diluted with oil according to specified directions and, when so diluted, are much less expensive than ready-to-use solutions. Manufacturers' directions should be followed implicitly. Both solutions may be purchased through local hardware or retail lumber yards. A partial list of manufacturers and distributors of such preservatives is included in the Appendix. A solution containing 5% by weight of pentachiorophenol or a copper naphthenate solution containing 2% by weight of copper metal is recommended for wood in contact with the ground. Stove oil and the lighter diesel oils are good diluents because of their low viscosities at normal temperatures. Used crankcase oil has also been employed as an inexpensive diluent. Lighter oils, such as Stoddard's solvent and mineral spirits, are used as solvents for preservatives and water repellants for dip treatments, but they are more expensive and more volatile than the other oils. All oils are inflam- mable and adequate precautions should be taken to reduce fire hazard. Copper naphthenate is green in color and the depth of treatment is readily apparent on split surfaces of the wood. Pentachlorophenol is only slightly visible, but dyes can be added to color the solution. A red dye has been found to color the wood satisfactorily when added in the proportions of 1 grams (about 1 teaspoonful) to each gallon of treating solution. Any dye that forms a true solution and colors the wood distinctly is satisfactory. - See selected list of references in Appendix. t A product of the Portland Gas and Coke Company, Public Service Bldg., Portland 4, Oregon. Sudan Red BBA Dye, R 5586, General Dyestuff Corporation, San Francisco, California; cost about $1.80 per pound. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 19 Precautions recommended by the manufacturer should be observed when handling wood preservatives. Their general recommendations are to avoid contact with the skin and prolonged breathing of the vapors. Washing with soap and water within a reasonable length of time after handling treated posts has been found to be an effective precautionary measure. Individuals who develop skin irritations should wear oil-resistant gloves and aprons. Purchasers of preservatives should beware of claims as to exceptional penetration or toxic properties. Demonstrations using dry, easily penetrated wood cannot be considered typical of material usually treated. A good practice is to buy from reputable dealers those preservatives whose compositions are clearly described on the label of the container. Control of treatment The amount of preservative retained by the posts can be measured by weighing the posts before and after treatment or by noting the amount of preservative that must be added to the treating tank to maintain a given depth. Retention, however, is not necessarily a reliable indication of the effectiveness of the treatment; good distribution of the preservative is even more important. Distribution of the preservative can be determined by increment borings, by drilling holes in the posts with a brace and bit and noticing the depth at which untreated wood is encountered, or by actually splitting test posts. If either of the first two methods is used, the holes should be plugged with treated pegs or dowels. The third method, even though it necessitates the destruction of a few posts, gives a better picture of the distribution of preserva- tive in the post. The posts or post sections to be cut should be typical of the charge and comparatively free of large knots, scars, or cuts that expose end grain; such features could produce an erroneous indication of the average treatment. The entire post may be split, or the post may be crosscut into sections that may then be split with the grain. The split faces should be examined immediately, for the oil creeps over the cut surfaces, giving a false indication of the depth and uniformity of treatment. Treating standards Since the ground-line zone and the ends of the posts are the critical post sections from the standpoint of initial attack by wooddestroying organisms, the protection of these sections is of primary importance. The sapwood of the ground-line section should be treated uniformly and as deeply as possible. The sapwood at each end of the 20 INFORMATION CIRCULAR 4 post should be completely penetrated for several inches and the heartwood should have some penetration. The importance of securing a uniform treatment, as illustrated in the frontispiece, cannot be overemphasized. Although the treatment should attempt to provide a retention of 6 pounds of preservative for each cubic foot of wood, it may be impossible to obtain this retention with many species. However, longer soaking periods will improve both the retention and the uniformity of the treatment. Cost of treating solution The costs of the treating solution may vary from about 1.20 per gallon for ready-to-use solutions to $0.45 per gallon for the concen- trate form diluted with diesel oil. The following formula may be used for computing the cost of the treating solution: Cost of one gallon Cost of oil added or one pound of + to dilute the concentrate concentrate Cost of treating = solution per Gallons or pounds of treating solution gallon or pound For example, the cost of 1 gallon of a 1 to 10 treating solution made from pentachlorophenol concentrate at $3.50 per gallon and diesel oil at $0.14 per gallon would be as follows: $3.50+ (10 >( $0.14) - $0.45 per gallon (or $0.065 per pound) 11 The cost of preservative for treating posts of various sizes to a retention of 6 pounds per cubic foot is shown in Table 2. Table 2. ESTIMATED COSTS FOR TREATING POSTS OF VARIOUS SIZES Post diameter Approximate cost per linear foot Inches 4 34c 6 8 7.6 13.6 12 306 Since the highest retention that can be obtained for a number of species shown in Table 1 will be about 3 pounds per cubic foot, the cost of treatment will be greatly reduced for these species. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 21 Considerable Care should be exercised to avoid overtreatment and the resulting high costs when treating species that will take high retentions. Both overtreatment and undertreatment can be avoided through incising which, in many ways, is the key to successful preservative treatment of wood. The amount of solution remaining in the tank should be con- sidered when estimating the treating cost for a limited number of posts. Unless a large amount of material is to be treated, soaking can be an expensive treating method. HANDLING PRESERVATIVE-TREATED POSTS The value of a preservative treatment may be greatly reduced through improper handling practices or other abuses which expose untreated wood. Common abuses of treated posts include handling the posts with pointed instruments, cutting or boring through the treated layer, and burning. Sharpening the ends of posts or framing should, if possible, be done before the posts are treated. If the post must be cut after treatment, the exposed area should be swabbed heavily with the preservative solution. Cutting the treated wood at or below the ground line should be avoided. ADVANTAGES OF PRESERVATIVE-TREATED POSTS The following advantages of treated posts should be considered when comparing the costs of treated and untreated posts. Service life should be 15 years or longer; 30 years is not exceptional for pressure-treated posts. Maintenance costs are reduced because of long service life and the elimination of early failures. Smaller posts may be used to reduce initial, installation, and maintenance costs. Appearance of property is improved. Posts may be re-used with much less danger of breakage. Farm woodland timber can be utilized to better advantage because species of low natural durability may be used successfully when treated. 22 INFORMATION CIRCULAR 4 APPENDIX THE ACTUAL OR ESTIMATED SERVICE LIFE OF UNTREATED POSTS THAT HAVE BEEN OR ARE BEING TESTED IN THE T. J. STARKER POST FARM* Average Service Life of at Least 20 Years Cedar, Alaska split split split Cedar, Port Orford Cedar, Western red Juniper, 'Western Locust, black round and split round and split round and split Osage-orange Redwood Yew, Pacific sawed round Average Service Life of 10 to 15 Years Cedar, incense split split Oak, Oregon white Average Service Life of Less than 10 Years Alder, red Ash, Oregon Cascara Cottonwood, black Cypress, Arizona Douglas fir Fir, grand Hemlock, West coast Larch, western Madrone, Pacific Maple, Oregon Pine, lodgepole Pine, ponderosa Pine, sugar Pine, Idaho white Spruce, Sitka Tanoak V ears split split round split round round and sawed split sawedsawed round and split split round sawed sawed sawed sawed round 5 6 3 5 4 4 9 6 7 6 6 4-5 6 7 6 6 5 The T J. Starker Post Farm was established by the School of Forestry, Oregon State College, in 1927 to determine the durability of native woods and the effectiveness of various preservative treatments. It is now under the supervision of the Oregon Forest Products Laboratory in cooperation with the School of Forestry. Annual progress reports on the Post Farm are available, free of charge. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 23 SELECTED REFERENCES ON WOOD PRESERVATION General J. 0. Wood Preservatives. Report No. R149. U. S. Forest Products Laboratory. Revised 1953 *BIeW, Bonnicksen, L. W., Graham, R. D., and Huber M. 0. Pole-frame Cot3 4. 5 struction. Circular 559. Extension Service, Oregon State College, Corvallis. (Free of charge.) September 1953. *Hunt, G. M. Making Log Cabins Endure. Report No. R982. U. S. Forest Products Laboratory. Revised 1950. Hunt, G. M., and Garratt, G. A. Wood Preservation. Second Edition. McGraw-Hill Book Company, Inc. New York, 1953. *Li.s. of Publications on Wood Preservation. Report No. 704. U. S. Forest Products Laboratory. March 1954. Manual of Recommended Practices. American Wood-Preserver's Association, 839 Seventeenth Street, N. W., Washington 6, D. C. Preventing Damage to Buildings by Subterranean Termites, and Their Control. Farmers' Bulletin No. 1911, U. S. Department of Agriculture. (From Superintendent of Documents, Government Printing Office, Wash- ington 25, D. C., for 10 cents.) * Treating Spruce and Balsam Fir Christmas Trees to Reduce Fire Hazard. Technical Note No 250. U. S. Forest Products Laboratory. Wood Preservation (A guide to the specification and use of pressure processes for Douglas fir and other western woods). Western Wood Preserving Operators' Association, 1410 S. W. Morrison Street, Portland 5, Oregon. Treating Methods *Baechler, R. H. How to Treat Fence Posts by Double Diffusion. Report No. 1955, U. S. Forest Products Laboratory. September 1953. *Blew, J. 0. Treating Wood in Pentachlorophenol Solutions by the Coldsoaking Method. Report No. R1445, U. S. Forest Products Laboratory. Revised 1950. Colleary, M. J. The Preservative Treatment of Fence Posts by Nonpressure Processes. Forestry Branch Bulletin No. 107, Forest Products Laboratory, Ottawa, Canada. MacLean, J. D. Preservative Treatment of Wood by Pressure Methods. Handbook No. 40, U. S. Department of Agriculture. (From Superintendent of Documents, U. S. Gov. Printing Office, Washington 25, D. C., for 40 cents.) December 1952. *Methods of Applying Wood Preservatives. Report No. R154, U S. Forest Products Laboratory. Revised 1953. *Preservatjve Treatment of Fence Posts and Farm Timbers. Farmers' Bulletin No. 2049, U. S. Department of Agriculture. September 1952. Salt Treatment for Green Posts and Poles. Circular 556, Extension Service, Oregon State College, Corvallis. (Free of charge.) July 1953 May be obtained free of charge by writing the Director, Ii. S. Forest Products Laboratory, Madison 5, Wisconsin. 24 INFORMATION CIRCULAR 4 *Wirka, R. M. Preservation of Timber by the Steeping Process. Report No. R621, U. S. Forest Products Laboratory. Revised December 1945. Wohlez, E., and Ravenscroft, V. Cold-soak Wood Preservation. Extension Bulletin No. 187, College of Agriculture, University of Idaho, Moscow, Idaho. (Free of charge.) June 1951. Durability and Serviceability *Blew, J. 0. Comparison of Wood Preservatives in Stake Tests (Annual Progress Report.) Report No. R1761, U. S. Forest Products Laboratory. 1954. *Blew, J. 0., and Kulp, J. W. Comparison of Wood Preservatives in Mississippi Post Study (Annual Progress Report). Report No. 1757, U. S. Forest Products Laboratory. 1954. Graham, R. D. Service Life of Treated and Untreated Fence Posts. Progress Report 8, Oregon Forest Products Laboratory, Corvallis. (Free of charge.) October 1954. *Hunt, G. Factors that Influence the Decay of Untreated Wood in Service and Comparative Decay Resistance of Different Species. Report No. R68, U. S. Forest Products Laboratory. 1941. THE SOAKING METHOD FOR PRESERVING FENCE POSTS 25 PARTIAL LIST OF MANUFACTURERS AND DISTRIBUTORS OF COPPER NAPHTHENATE AND PENTACHLOROPHENOL Trade Name Manl4facturer Distribittor COPPER NAPHTHENATE General Petroleum Corp. 710 NE Holladay Portland 14, Oregon Copper Naphthenate General Petroleum Corp. 710 NE Holladay Portland 14, Oregon Nuodex Products Ca, Inc. Elizabeth F, New Jersey Nuodex Copper Fred E Alsop Company Oronite Chemical Company 200 Bush Street San Francisco 20, Calif. Oronite Copper Van Waters & Rogers, Inc. Wood Treating Chemicals Co. 5137 Southwest Avenue St Louis 10, Missouri 935 N. W. 12th Avenue Portland 9, Oregon Naphthenate (8%) 3950 N. W. Yeon Avenue Portland 10, Oregon Coppertreat Wood Treating Chemicals Co. Public Service Bldg. 920 S. W. Sixth Avenue Portland 4, Oregon Penta Preservative Chapman Chemical Co. Kenite L. H. Butcher Company 1504 N. W. Johnson St. Portland 9, Oregon PENTACHLOROPHENOL Chapman Chemical Company Terminal Sales Building Portland 5, Oregon Gilbreath Chemical Co 383 Brannan Street San Francisco, Calif. Miller Products Company Ft. of S. W. Caruthers Portland 1, Oregon Monsanto Chemical Co. Organic Chemicals Div. St. Louis 4, Missouri Terminal Sales Building Portland 5, Oregon Miller's Penta Miller Products Company Ft. of S. W. Caruthers Portland 1, Oregon Monsanto Penta Monsanto Chemical Co. 911 Western Avenue Seattle 4, Washington Pacific Supply Cooperative 1928 N W. Vaughn Street Portland 8, Oregon Co-op Wood Preservative Pacific Supply Cooperative 1928 N. W. Vaughn Street Portland 8, Oregon Protection Products Mfg. Co. Kalamazoo, Michigan Woodlife Woodhealth Chas. E Sand Plywood Co. 1106 N. W. 16th Avenue Portland 9, Oregon Wood Treating Chemicals Co. 5137 Southwest Avenue St. Louis 10, Missouri Timbertox Woodtox Wood Treating Chemicals Co. Public Service Bldg. 920 5. W. Sixth Avenue Portland 4, Oregon Builterials Company 2350 N. W. St. Helens Rd. Portland 10, Oregon Penta Stain 26 INFORMATION CIRCULAR 4 Distributor Trade Name Manufacturer Van Waters & Rogers, Inc. 3950 N. W. Yeon Avenue Portland 10, Oregon Guardsman Van Waters & Rogers, Inc. 3950 N. W. Yeon Avenue Portland 10, Oregon COMMERCIAL WOOD PRESERVING PLANTS IN OREGON* Company Baxco Corporation 541 Pittock Block Portland 5 Plant Address Type of Treatment The Dalles Pressure J. H. Baxter & Co. of Oregon Pressure 541 Pittock Block Portland 5 Koppers Company, Inc. 370 Pittock Block Portland 5 McCormick & Baxter Creosoting Company P. 0. Box 3344 Portland 8 L. D. McFarland Co., Ltd. P. 0. Box 752 Eugene Pressure P. 0. Box 166 Wauna Pressure Nonpressure (cedar poles) 6900 North Edgewater P. 0. Box 2648 Portland 3 Nonpressure Highway 99N Eugene P. 0. Box 445 Eugene Pope and Talbot, Inc. Wood Preserving Department 3070 N. W. Front Avenue Portland 10 Pressure St. Helens Assistance in the use of pressure.treated material can be obtained from \V. R. Bond, Engineer, Service Bureau, American Wood.Preservers' Association, 1410 S. V. Morrison St., Portland 5, Oregon.